• Mass or block polymerization: Polymerization of the
• carried out by adding a soluble initiator to
pure monomer (in liquid state).
• The mixture is constantly agitated & heated to
• Once the reaction starts, heating is stopped as the
reaction is exothermic.
• The heat generated is dissipated by circulating water
• Viscosity increases dramatically during conversion.
• The method is used for the polymerization of liquid
• It is usually adopted to produce polystyrene,
polyvinyl chloride, polymethyl methacrylate and low
• The system is simple and
requires thermal insulation.
• The polymer is obtained pure.
• Large castings may be
• Molecular weight
distribution can be easily
changed with the use of a
chain transfer agent.
• Heat transfer and mixing
become difficult as the
viscosity of reaction mass
• Highly exothermic.
• The polymerization is
obtained with a
broad molecular weight
distribution due to the
high viscosity and lack of
good heat transfer.
• Very low molecular weights
Some disadvantages of bulk polymerization are
eliminated in solution polymerization.
Monomer along with initiator dissolved in solvent,
formed polymer stays dissolved.
The mixture is kept at polymerizaion temperature &
Depending on concentration of monomer the viscosity
of solution does not increase.
After the reaction is over, the polymer is used as such
in the form of polymer solution or the polymer is
isolated by evaporating the solvent.
Polymer so formed can be used for surface coating.
It is used for the production of Polyacrylonitrile, PVC,
Polyacrylic acid, Polyacrylamide, Polyvinyl alcohol,
PMMA, Polybutadiene, etc
• The solvent acts as a diluent & helps in facilitating
continuous transfer of heat of polymerization.
Therefore temperature control is easy.
• The solvent allows easy stirring as it decreases the
viscosity of reaction mixture.
• Solvent also facilitates the ease of removal of polymer
from the reactor.
• Viscosity build up is negligible.
• To get pure polymer, evaporation of solvent is required
additional technology, so it is essential to separate &
recover the solvent.
• The method is costly since it uses costly solvents.
• Polymers of high molecular weight polymers cannot be
formed as the solvent molecules may act as chain
• The technique gives a smaller yield of polymer per
reactor volume, as the solvent waste the reactor space.
• The purity of product is also not as high as that of bulk
polymerization. Removal of last traces of solvent is
Liquid or dissolved monomer suspended in liquid
phase like water.
Initiators used are monomer soluble e.g. dibenzoyl
Thus, polymer is produced in heterogeneous medium.
The size of monomer droplets is 50-200 μm in
The dispersion is maintained by continuous agitation
and the droplets are prevented to coalesce (unite or
merge) by adding small quantity of stabilizers.
The stabilizers used are PVA, gelatin, cellulose are
used along with inorganic stabilizers such as kaolin,
magnesium silicate, aluminum hydroxide,
calcium/magnesium phosphate, etc if necessary.
As it concerns with droplets, each droplet is tiny bulk
reactor. The polymerization takes place inside the
droplet & product formed being insoluble in water.
The product separated out in the form of spherical
pearls or beads of polymer.
Hence the technique is also known as Pearl
polymerization / Granular polymerization / Bead
The products are small uniform spheres. They can be
used directly for some applications as precursors of
ion exchange resins otherwise they can be extruded &
chopped to form larger, easily moulded pallets.
They can be dissolved in a suitable medium for use as
adhesives & coatings.
This technique is used to form PVC, Polyvinyl
acetate, Polystyrene, Styrene-divinyl benzene
copolymer beads (used for ion exchange) etc.
• The process is comparatively cheap as it involves only
water instead of solvents.
• Viscosity increase is negligible.
• Agitation & temperature control is easy.
• Product isolation is easy since the product is insoluble
• The method can be adopted only for water insoluble
• It is difficult to control polymer size.
• Polymer purity is low due to the presence of suspending
& stabilizing additives that are difficult to remove
• Suspension polymerization reaction is highly agitation
• Larger volume of reactor is taken up by water.
• The method cannot be used for tacky polymers such as
elastomers because of the tendency for agglomeration of
The technique is used for the production of large
number of commercial plastics & elastomers.
The system consists of water insoluble monomer,
dispersion medium & emulsifying agents or
surfactants (soaps and detergents) and a water soluble
initiator (potassium persulphate / H2O2, etc).
The monomer is dispersed in the aqueous phase, not
as a discrete droplets, but as a uniform emulsion.
The size of monomer droplet is around 0.5 to 10 μm
in diameter depending upon the polymerization
temperature & rate of agitation.
The emulsion of monomer in water is stabilized by a
A surfactant has a hydrophilic and hydrophobic end in
When it is put into a water, the surfactant molecules
gather together into aggregates called micelles.
The hydrocarbon tails (hydrophobic) orient inwards &
heads (hydrophilic) orient outwards into water.
The monomer molecules diffuse from monomer
droplets to water & from water to the hydrocarbon
centre of micelles.
fast polymerization rates.
allows removal of heat from
viscosity remains close to
that of water and is not
dependent on molecular
The final product can be used
as such ,does not need to be
altered or processed
Surfactants and polymerization
adjuvants -difficult to remove
For dry (isolated) polymers,
water removal is an energy-intensive
Designed to operate at high
conversion of monomer to
polymer. This can result in
significant chain transfer to
Can not be used for
condensation, ionic or Ziegler-